Modulated structure and phase transitions of Sr~10~Ga~6~O~19~
Krüger, Hannes; Lazić, Biljana; Arroyabe, Erik; Kahlenberg, Volker; Acta Crystallographica Section B 65 (2009) 587–592; doi:10.1107/S0108768109026974

data_2104467
_publ_section_title
;
 Modulated structure and phase transitions of Sr~10~Ga~6~O~19~
;
_journal_coeditor_code           SN5086
_journal_issue                   5
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              587
_journal_page_last               592
_journal_paper_doi               10.1107/S0108768109026974
_journal_volume                  65
_journal_year                    2009
_chemical_formula_sum            'Ga6 O19 Sr10'
_chemical_formula_weight         1598.5
_chemical_name_systematic        ' ?'
_space_group_ssg_name            C2/c(0\b0)s0
_symmetry_cell_setting           monoclinic
_audit_creation_method
;
  Jana2000 Version : 18/12/2007
  STOE X-RED
  enCIFer 1.3
;
_cell_angle_alpha                90
_cell_angle_beta                 103.551(3)
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   34.9145(13)
_cell_length_b                   7.9369(2)
_cell_length_c                   15.9150(7)
_cell_measurement_reflns_used    21142
_cell_measurement_temperature    298
_cell_measurement_theta_max      27.33
_cell_measurement_theta_min      1.31
_cell_modulation_dimension       1
_cell_volume                     4287.5(3)
_computing_cell_refinement       'STOE X-AREA'
_computing_data_collection       'STOE X-AREA'
_computing_data_reduction        'STOE X-RED'
_computing_molecular_graphics    DRAWxtl
_computing_publication_material
'Jana2000 (Petricek, Dusek & Palatinus, 2000)'
_computing_structure_refinement
'Jana2000 (Petricek, Dusek & Palatinus, 2000)'
_diffrn_ambient_temperature      298
_diffrn_detector_area_resol_mean 6.67
_diffrn_measured_fraction_theta_full 0.98
_diffrn_measurement_device       '2-circle goniometer'
_diffrn_measurement_device_type  'STOE IPDS 2'
_diffrn_measurement_method       'rotation method'
_diffrn_radiation_monochromator  'plane graphite'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0707
_diffrn_reflns_av_sigmaI/netI    0.0641
_diffrn_reflns_limit_h_max       42
_diffrn_reflns_limit_h_min       -42
_diffrn_reflns_limit_index_m_1_max 1
_diffrn_reflns_limit_index_m_1_min -1
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            47585
_diffrn_reflns_reduction_process
; STOE X-AREA/INTEGRATE 1.39
  elliptical profiles, parameters A=11.1,B=2.9,EMS=0.057
  5% overlap tolerance
  q-vector profile factor 0.8
;
_diffrn_reflns_theta_full        25.87
_diffrn_reflns_theta_max         25.87
_diffrn_reflns_theta_min         1.20
_exptl_absorpt_coefficient_mu    32.134
_exptl_absorpt_correction_T_max  0.188
_exptl_absorpt_correction_T_min  0.065
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details
'(Jana2000; Petricek, Dusek & Palatinus, 2000)'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    4.9512
_exptl_crystal_description       fragment
_exptl_crystal_F_000             5741
_exptl_crystal_size_max          0.200
_exptl_crystal_size_mid          0.140
_exptl_crystal_size_min          0.100
_refine_diff_density_max         5.43
_refine_diff_density_min         -4.45
_refine_ls_extinction_coef       204E1(11)
_refine_ls_extinction_method
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_goodness_of_fit_ref   2.65
_refine_ls_number_parameters     947
_refine_ls_number_reflns         15579
_refine_ls_R_factor_all          0.1383
_refine_ls_R_factor_gt           0.0840
_refine_ls_shift/su_max          0.0005
_refine_ls_shift/su_mean         0.0000
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(\s^2^(F)+0.0001F^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0677
_refine_ls_wR_factor_ref         0.0734
_reflns_number_gt                10533
_reflns_number_total             15579
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            sn5086.cif
_cod_data_source_block           RTmod
_cod_depositor_comments
;
The following automatic conversions were performed:
'_exptl_absorpt_correction_type' value 'Gaussian' changed to 'gaussian'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 

The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Gaussian' changed to
'gaussian' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_database_code               2104467
_cod_database_fobs_code          2104467